electric glue: electrically controlled polymer-surface ... the stretching of the polymer chain prior
Post on 05-Jul-2020
Embed Size (px)
Published: April 26, 2011
r 2011 American Chemical Society 1993 dx.doi.org/10.1021/nl200353h |Nano Lett. 2011, 11, 1993–1996
Electric Glue: Electrically Controlled Polymer-Surface Adhesion Ann R. Fornof,*,† Matthias Erdmann,† Ralf David,‡ and Hermann E. Gaub*,†
†Chair for Applied Physics and Center for Nanoscience, Ludwig-Maximilians University, Amalienstrasse 54, Munich, Germany 80799 ‡Center for Integrated Protein Science Munich, Butenandtstrasse 5-13, Munich, Germany 81377
bS Supporting Information
Electric potential has been used to attract polymers continu-ously to an electrode surface and to toggle molecules between states for a molecular switch.2�4 For electric glue, the focus is to control the interaction of a polymer and an electrode surface reversibly, thus creating a nanoscale system with electro- chemically controlled adhesion (Figure 1a). The reversible bonding of an organic molecule, DNA, to an inorganic surface, a gold electrode, was recently accomplished by varying the electric potential of the surface, and the interaction was measured via atomic force microscopy (AFM).1 In the current work, control over electrosorption, or covalent bonding with the sur- face based on potential, is extended and refined to include physisorption, or noncovalent interaction between the polymer and the surface. The manipulation of the interaction and reaction of polymers from commercially available to tailored macromo- lecules with a surface is described.
To explore this concept further, we utilized a custom AFM setup with a working electrode as the surface of interest (Figure 1b). The polymers were covalently attached to the AFM tip and brought into contact with the surface of a gold working electrode at a specified potential. As the polymers were removed from the electrode in the z-direction, the resultant force was measured, and the potential of the electrode was changed by 10 mV. The potential of the electrode regulated oxidation/ reduction reactions at the surface of the electrode.5
While the Au�S bond is the most studied bond for organic modification of gold surfaces, it has a bond strength close to that of the Au�Au bond.6,7 Therefore, it is difficult to distinguish experimentally between Au�Au and Au�S bond rupture, and reversible attachment/detachment would be unpredictable due to the possibility of pulling gold nanowires from the surface of the electrode.8 Therefore, the targeted bond for reversible
attachment was the dative, N�Au bond. The tip-attachment chemistry and polymeric chemistry were designed such that the N�Au bond was the weakest bond in the construct. For the N�Au reaction, the amine donates both electrons from its lone pair to share with undercoordinated gold in a classic example of a dative bond.9,10
Three polymers with differently charged backbones and primary amine end groups were utilized to control adhesion based on the electric potential of the surface, as well as to probe the influence of backbone charge on this process, in this series of experiments. Figure 1a depicts the experiment for the positively charged polymer. The same experimental setup was used for each of the experiments with polymers of differing backbone charge.
In each experiment, a different backbone charge on the polymer was explored by using an AFM tip functionalized with a different polymer. The neutral polymer chosen was poly- (ethylene glycol) (PEG-NH2), a commercially available poly- mer; a 2,2-ionene, which was synthesized in-house (Supporting Information Figure S1), was selected for the positively charged backbone and finally, a biopolymer, double-stranded DNA, where three of the four bases contain primary amines, was used as the negatively charged polymer. Strong polyelectrolytes, whose charge in solution does not change substantially under moderate pH conditions, were chosen so that the polymeric backbone charge would remain the same at the bulk pH as well as the expected pHs local to the electrode surface.11 A 2:1 electro- lyte solution of 50 mMMgCl2 at pH 8.5 provided an ambient for the dsDNA such that it would remain double-stranded and the
Received: January 29, 2011 Revised: April 13, 2011
ABSTRACT: Polymer-surface interactions provide a basis for nanoscale design and for understanding the fundamental chemistry and physics at these length scales. Controlling these interactions will provide the foundation for further manipulation, control, and measurement of single molecule processes. It is this direction of control over nanoscale polymer-surface interactions that we explore with electric glue. The adhesion between surfaces and single molecules is manipulated based on an externally controlled potential in electric glue.
KEYWORDS: Single-molecule force spectroscopy, polymers, atomic force microscopy, electrochemistry
1994 dx.doi.org/10.1021/nl200353h |Nano Lett. 2011, 11, 1993–1996
Nano Letters LETTER
primary amines deprotonated. The same solution composition was utilized throughout the experiments with one exception. The no salt ionene experiment was performed without added MgCl2.
The neutral backbone of the PEG-NH2 allowed for explicit examination of the N�Au bond. At static potential but varied loading rates, the force followed the expected behavior for covalent bond rupture (Supporting Information Figure S2).13
The stretching of the polymer chain prior to rupture observed in the force curves indicated that the polymer was pinned at its end group (Supporting Information Figure S3).14,15 Control experiments with PEG and a methoxy end group showed no interaction between the polymer and the surface (data not shown).
Under dynamic potential, the force to remove the polymer from the surface was determined as the potential was cycled from 1 to �1 V via an externally controlled potentiostat (Figure 2a). The change in potential is shown in Figure 2a, and the rupture force under those potential conditions is shown in Figure 2b�e. After each force curve, the potential was changed by 0.01 V and a curve number assigned to the force curve at that potential. The data in the graph was binned such that each bar in the graph represents ten force curves. Because of the binning of the data, the absolute forces measured can reflect in part the likelihood of a successful N�Au bonding event. A high-tip functionalization density was used to prolong the longevity of the experiment.
Over several hundred or thousand force curves the functionaliza- tion of the tip was observed to decrease (see, for example, Figure 2e); this tip wear-out may have been due to mechanical damage to the tip over these long experiments. However, the last rupture event in the force curve was measured, and thus, only single polymer events were recorded. The small potential steps minimized artifacts due to ion currents acting on the cantilever.
The data is plotted in a roburogram (robur is Latin for force), where the rupture force is plotted versus potential. This plot is akin to the cyclic voltammogram (Figure 3a) except that the y-axis is the rupture force rather than current (Figure 3b�d). The adhesion of PEG-NH2 was reduced at the highest and lowest potential regimes explored and was only moderately sensitive to the direction of charging as indicated by the slight hysteresis in the roburogram at potentials around 0.3 to 0.5 V (Figure 3b). Near the potential extremes (1 or �1 V), there was negligible interaction between the polymer and the surface. The reversible electrosorption of PEG-NH2 was observed for over 2000 force curves; thus demonstrating the longevity and reproducibility of the adsorption (Supporting Information Figure S4).
The PEG-NH2 provided a baseline for the behavior of the N�Au reaction and demonstrated the control possible over electrosorption of the N�Au bond based on the applied potential to the surface. The polymers could then be tailored to exert control over the physisorption through the introduction of charge to the polymer backbone in combination with electro- sorption due to the coordinate N�Au bond.
Rather than the polymer interacting with the electrode under all potential conditions except at the extreme potentials, as was the case for PEG-NH2, the amine-end-capped ionene with its positively charged backbone began reacting with the surface at potentials close to 0.3 V only when the potential was ramped down from 1 V. However, there was negligible interaction between the polymer and the working electrode surface in the reverse direction (Figure 3d).
A strong hysteresis was also observed for the potential- dependent interaction of dsDNA with the gold electrode. Three of the four nucleotides that are found in DNA contain primary amine functionality, that is, adenine, guanine, and cytosine; only thymine does not have a primary amine moiety (Supporting
Figure 1. The experimental setup. (a) Throughout the electrochemical cycle from 1 to �1 V, the gold, working electrode surface undergoes oxidation and reduction and magnesium ions (shown in orange) from solution are attracted to the surface under certain potential ranges. The charged polymer responds to the surface chemistry of the electrode, ion concentration, and the availability of undercoordinated, reactive gold sites (shown in green). Under the appropriate conditions, the amine end group reacts with the gold surface, and the reactive surface is refreshed throughout the cycle, and the adhesion repeatedly occurs at the same potential ranges and is also turned off repeatedly. (b) The three electrode electrochemical cell used is comprised of a gold working electrode, a Ag/AgCl reference electrode, and a platinum counter electrode.